M A S O N R Y I N F O R M A T I O N
Centuries ago, combinations of sand and lime were used as
mortar.These combinations took months and even years to harden, as
thelime slowly combined with carbon dioxide from the air to
formcalcium carbonate. Because it took so long for these mortars
toharden and gain strength, it was necessary to use very thin
joints.In many instances the joints were so thin that adjacent
masonry unitswould bear on each other in direct contact. This type
of constructionrequired an excessive amount of labor to carefully
fit and place eachmasonry unit. However, sand-lime mortars were
adequate for the thenmassive construction and slow-paced
The development of mortars that harden and gain strength
rapidlymade it possible to place masonry units quickly. Also,
thicker jointsprovided cushions for dimensional variations in the
masonry units.The stronger mortars were first obtained by
"sweetening" the limewith a small amount of portland cement. Later,
the ratio of portlandcement was progressively increased until the
process involved sweeteningthe cement with a small amount of
In the later 19th century, the advancement of strong mortars
withcontrolled setting characteristics was a major step forward for
masonryconstruction. Another important step was the development of
masonrycements in the 1930s.
Masonry cement is factory-prepared hydraulic cement primarily
usedto produce masonry mortar or portland cement plaster
(stucco).Masonry cement consists of a mixture of portland or
blendedhydraulic cement and plasticizing materials (such as
limestone,hydrated, or hydraulic lime) together with other
materials introducedto enhance one or more properties such as
setting time, workability,water retention, and durability. White
masonry cement and coloredmasonry cements containing premixed
mineral oxide pigments arealso available in many areas. All are
mixed and packaged underfactory conditions, increasing quality
Today, most mortars are made with masonry cement due to the
easeof use and consistent performance. These mortars are a
combinationof a masonry cement, clean and well-graded sand, and
enough cleanwater to produce a plastic, workable mix. Masonry
cements aredesigned to ease the mixing operation at the
construction site. Theiruse produces color and batch uniformity.
Masonry cements that
meet the requirements of American Society for Testing and
Materials(ASTM) designation C 91 or Canadian Standards Association
(CSA)standard A3002 ensure workable, sound, and durable mortar.
In the 1990s, increased use of masonry in demanding
structuralapplications and high seismic areas resulted in the
development of a new product, mortar cement. Mortar cement is
similar to masonrycement in that it is a factory-prepared hydraulic
cement primarilyused to produce masonry mortar. However, ASTM C
1329, theStandard Specification for Mortar Cement, places lower
maximum air content limits on mortar cement than permitted for
masonrycements, and ASTM C 1329 is the only ASTM masonry
materialspecification that includes bond strength performance
Mortar for masonry is designed not only to join masonry units
intoan integral structure with predictable performance properties,
butalso to: (1) effect tight seals between units against the entry
of airand moisture; (2) bond with steel joint reinforcement, metal
ties, andanchor bolts, if any, so that they perform integrally with
the masonry;(3) provide an architectural quality to exposed masonry
structuresthrough color contrasts or shadow lines from various
joint-toolingprocedures; and (4) compensate for size variations in
the units byproviding a bed to accommodate tolerances of units.
Masonry mortar is composed of one or more cementitious
materials;clean, well-graded masonry sand; and sufficient water to
Fig. 1. Mortar of proper workability is soft, but with good
body;it spreads readily and extrudes without smearing
or dropping away. (IMG13629)
plastic, workable mixture. Modern specifications call for
proportionsby volume ranging from one part of cementitious material
to 21⁄4 to31⁄2 parts of damp, loose mortar sand. The choice of
cementitiousmaterial—masonry cement, mortar cement, a portland
cement andlime combination, or a portland cement and masonry
cementor mortar cement combination—is largely a matter of
economicsand convenience. Any of these combinations will produce
mortarwith acceptable properties as long as applicable
specifications aremet and appropriate design procedures are
Good mortar is necessary for good workmanship and proper
structuralperformance of masonry construction. Since mortar must
bondmasonry units into strong, durable, weathertight walls, it must
havethe properties described below.
Workability. Probably the principal quality of plastic
masonrymortar is workability, because of its influence on other
importantmortar properties in both the plastic and the hardened
states.Workability is difficult to define because it is a
combination of anumber of interrelated properties. The properties
considered as havingthe greatest influence on workability are
consistency (flowability),water retentivity, setting time, weight,
adhesion, and cohesion.
An experienced mason judges the workability of mortar by the way
itadheres to or slides from his trowel. Mortar of good workability
shouldspread easily on the masonry unit, cling to vertical
surfaces, extrudereadily from joints without dropping or smearing,
and permit easypositioning of the unit without subsequent shifting
due to its weightor the weight of successive courses. A mortar's
consistency should becompatible with the units and weather
conditions. For example, underhot summer conditions when using a
high-absorption unit, a softermortar having a higher water content
is needed, compared to thatused with a dense unit during cold
Water retentivity. Mortar having this property resists rapid
loss ofmixing water (prevents loss of plasticity) to the air on a
dry day or to anabsorptive masonry unit. Rapid loss of water causes
the mortar to stiffenquickly, making it practically impossible to
obtain weathertight joints.
Water retentivity is an important property and is related to
workability.A mortar that has good water retentivity remains soft
and plasticlong enough for the masonry units to be carefully
aligned, leveled,plumbed, and adjusted to proper line without
danger of breaking theintimate contact or bond between mortar and
unit. When low-absorption units such as split block are in contact
with a mortar havingtoo much water retentivity, they may float.
Consequently, the waterretentivity of a mortar should be within
tolerable limits. Water addsworkability to the mortar; entrained
air or extremely fine aggregateor cementitious materials not only
add workability or plasticity to themortar, they also increase its
Consistent rate of hardening. The rate of hardening of a mortar
due to hydration (chemical reaction) is the speed at which
itdevelops resistance to an applied load. Rapid hardening may
interfere with the use of the mortar by the mason. Very slow
hardeningmay impede the progress of work, because the mortar will
extrudefrom the completed masonry. During winter construction, slow
hard-ening may also subject mortar to early damage from frost. A
well-defined, consistent rate of hardening assists the mason in
laying themasonry units and in tooling the joints at the same
degree of hardness.
Uniform color of masonry joints reflects proper hardening and
consistent tooling times. Hardening is sometimes confused with
astiffening caused by rapid loss of water, as when low-water
retentionmortar is used with highly absorptive units. Also, in very
hot, dryweather, mortar may tend to stiffen more rapidly than
usual. In thiscase, the mason may find it advisable to lay shorter
mortar beds andfewer units in advance of tooling. See also
"Hot-weather construction"of this publication.
Durability. The durability of masonry mortar is its ability to
endureexposure conditions. Mortar joints can deteriorate from
exposure tofreeze-thaw cycles when saturated, from exposure to
aggressivechemical environments, or from the use of unsound
Damage by frost action—either to mortar joints or to mortar
bond—has not been a problem in most masonry wall construction
abovegrade. In order for frost damage to occur, the hardened mortar
mustfirst be water-saturated or nearly so. Although mortar is
saturatedwhen first placed, the mixing water is absorbed by units
and chemicallycombined with cement compounds as the mortar hardens.
The saturatedcondition does not readily return except when the
masonry is in continuous contact with saturated soils, when
downspouts leak,when there are heavy rains, or when horizontal
ledges are formed.Under these conditions, the masonry unit and
mortar may becomesaturated, which can lead to freeze-thaw
deterioration if temperaturesdrop to freezing or below.
High-compressive-strength mortars usually have good
freeze-thawdurability. Because air-entrained mortar will withstand
hundreds offreeze-thaw cycles, its use provides good protection
against localizedfreeze-thaw damage. Masonry cement and mortar
cement mortarshave higher air contents than non-air-entrained
portland cement andlime mortar and therefore have better
freeze-thaw resistance. Mortarjoints that have deteriorated due to
freezing and thawing present amaintenance problem that usually
Sulfate attack provides an example where deterioration of
mortarresults from exposure to an aggressive chemical environment.
Sulfateresistance is usually not a concern for masonry above
ground;however, in some parts of the country, masonry can be
exposed tosulfate from soil, ground water, or industrial processes.
Sulfate-resistantmasonry materials should be used when they are
going to be in contact with soils containing more than 0.1%
water-soluble sulfate(SO4) or water solutions containing more than
150 ppm of sulfate.Without the use of sulfate-resistant masonry
units and mortar or use
of a protective treatment, sulfates would attack and
deterioratemasonry. Masonry cement, sulfate-resistant portland
cements (TypesII or V) or hydraulic cements (Types MS or HS), or
sulfate-resistantblended cements should be used in mortar exposed
to sulfates. Onestudy demonstrated that masonry cement is
significantly more sulfateresistant than a Type II portland cement
and lime mortar when testedin accordance with ASTM C 1012 (at 13
weeks, portland cement-lime mortars exhibited expansions of 0.16%
to 0.37% compared to0.03% to 0.12% for masonry cement mortars). For
additionalinformation see Dubovoy (1990).
Expansion in mortars due to unsound ingredients can cause
seriousdisintegration of masonry. Soundness of a hydraulically
cementitiousmaterial is measured by the autoclave expansion test
(ASTM C 151).This test produces reactions in unsound ingredients
(particularly freelime and periclase) and simulates a long period
of in-place exposure.ASTM specifications for masonry cement (ASTM C
91), mortarcement (ASTM C 1329), and portland cement (ASTM C 150)
limitacceptable changes in length of the test specimen to ensure
that noserious expansion of the hardened mortar will occur in a
wall. Whilea method for measuring soundness of hydrated lime has
been developed, correlation of results to field performance has not
yetbeen established. Thus, soundness is generally assured by
limiting theunhydrated oxide content of the hydrated lime to a
maximum of 8%.
Absorption of mortar is a measure of how much water the
hardenedmortar will take in. Low absorption mortars will be less
susceptibleto saturation, freeze-thaw deterioration, and staining.
Absoprtion isreduced by increasing cement content, using
air-entrained mortars,and using water repellent admixtures.
Compressive Strength. The principal factors affecting the
compressive strength of masonry structures are the
compressivestrength of the masonry unit, the proportions of
ingredients comprisingthe mortar, the design of the structure, the
workmanship, and thedegree of curing. Although the compressive
strength of masonry maybe increased with a stronger mortar, the
increase is not proportionalto the compressive strength of the
mortar. Tests have shown thatcompressive strengths of concrete
masonry walls increase only about10% when mortar cube compressive
strengths increase 130%.Composite wall compressive strengths
increase 25% when mortarcube compressive strength increases 160%
Compressive strength of mortar is largely dependent on the type
andquantity of cementitious material used in preparing the mortar.
Itincreases with an increase in cement content and decreases with
anincrease in air entrainment, lime content, or water content.
Portlandcement requires a period in the presence of moisture to
develop itsfull strength. To obtain optimum curing conditions, the
mortar mixtureshould contain the maximum amount of water compatible
withacceptable workability. Lean, oversanded mixtures should be
avoidedas they will have poor water retentive characteristics.
Freshly laidmasonry should be protected from the sun and drying
winds. Withsevere drying conditions, it may be necessary either to
wet theexposed mortar joints with a fine water spray daily for
about 3 daysor to cover the masonry with a plastic sheet, or
Bond. The term bond refers to a specific property that can be
sub-divided into: (1) extent of bond, or degree of contact of the
mortar withthe masonry units; and (2) bond strength, or force
required to separatethe units. A chemical and a mechanical bond
exist in each category.
Good extent of bond (complete and intimate contact) is important
towatertightness and tensile bond strength. Poor extent of bond at
themortar-to-unit interface may lead to moisture penetration
through theunbonded areas. Good extent of bond is obtained with a
workable andwater-retentive mortar, good workmanship, full joints,
and masonry unitshaving a medium initial rate of absorption
(suction). Bond strength isusually measured as tensile or flexural
bond strength. In determiningdirect tensile bond strength,
specimens representing unit and mortar arepulled apart (Fig. 3).
Test methods for measuring flexural (more properlytermed
“flexural-tensile”) bond strength place a more complex load onthe
mortar-to-unit interface, but can be applied to full-sized
Fig. 3. Tensile bond test. (IMG14591)
Fig. 2. Cube compressive-strength test. (IMG14091)
For example, ASTM Method C 1072 (Fig. 4) utilizes a bond
wrenchapparatus and loading configuration to induce failure of
prisms constructed from full-sized masonry units. Other standard
methodsused to measure bond strength of masonry include ASTM E 518,
ASTMC 952, and ASTM E 72. While bond strength is an important
propertyof masonry, current methods of test for determining bond
strength areconsidered impractical as a basis for material
specifications or qualitycontrol at the jobsite, due to the high
variability of results inherent inthe testing methods.
Many variables affect bond, including (1) mortar ingredients,
such astype and amount of cementitious materials, water retained,
and aircontent; (2) characteristics of the masonry units, such as
surface texture,suction, and moisture content; (3) workmanship,
such as pressureapplied to the mortar bed during placing; and (4)
curing conditions,such as temperature, relative humidity, and wind.
The effects of someof these variables on bond will be briefly
All other factors being equal, mortar bond strength is related
to mortar composition, especially the cement content. The
bondstrength of the mortar increases as the cement content
increases(Melander and Conway 1993).
Bond strength tends to decrease as air contents increase.
However,excellent bond strengths can be achieved using
air-entrained mortars.An extensive study of over 20 different
masonry cements representinga cross section of producers throughout
the United States confirmsthat masonry cements yield excellent
flexural bond strengths(Dubovoy and Ribar 1990). Seventy-five
percent of these masonrycement mortars tested with a brick unit
having an IRA* (initial rate ofabsorption) of 9 yielded bond
strengths in excess of 100 psi (690 kPa).None produced values lower
than 65 psi (450 kPa). The bondstrength criteria for mortar cements
were established to assurecomparable bond strength performance to
non-air-entrained portlandcement-lime combinations of equivalent
type designation (Melanderand Ghosh 1996).
Bond strength is low on smooth, molded surfaces, such as glass
ordie skin surfaces of clay brick or tile. On the other hand, good
bondis achieved on concrete block or on wire-cut or textured
surfaces ofclay brick. For high absorption clay brick, bond
strengths can beincreased by wetting the units prior to laying
them. However,surfaces of wetted brick should not be saturated.
Concrete masonryunits should not be wetted before use.
There is a distinct relationship between mortar flow (water
content)and bond strength. For all mortars, bond strength increases
as watercontent increases, within reasonable limits. The optimum
bondstrength is obtained by using a mortar with the highest water
contentcompatible with workability, even though mortar
compressivestrength may decrease (Isberner 1974a, Ritchie and
Workmanship is paramount in determining bond strength. The
timelapse between the spreading of mortar and the placing of
themasonry units should be kept to a minimum because the water
contentof the mortar will be reduced through suction of the masonry
unit onwhich it is first placed. If too much time elapses before
the upperunit is placed, the bond between the mortar and that unit
will bereduced. The mason should not realign, tap, or in any way
moveunits after initial placement, leveling, and alignment.
Movementdisrupts the bond between unit and mortar, after which the
mortarwill not reestablish good bond with the masonry units.
Volume change. As available water in mortar is absorbed by
themasonry units and lost through evaporation, some drying
shrinkageoccurs. Though generally not a problem in masonry
construction,extreme drying shrinkage can result in development of
cracks in themortar. Since drying shrinkage is related to the
amount of water lostby the mortar, factors that increase water
content of a mortar tendto increase its drying shrinkage. For
example, air-entrained mortarstend to have a lower water demand
than non-air-entrained mortarsat an equivalent flow and thus
exhibit less drying shrinkage.However, this principle should not be
misinterpreted to mean thatwater content of a mortar should be
arbitrarily reduced. As previouslynoted, workability and bond are
directly related to the flow of themortar and should be given
priority in determining the water contentof field mixed mortar.
On projects where it is desirable to minimize drying
shrinkage,masonry cement mortar should be considered. The shrinkage
of mortarcan be tested in accordance with ASTM C 1148. In a study
using thistest, masonry cement mortar had half the shrinkage of
cement-limemortar (0.07% at 25 days for masonry cement mortar
versus 0.12%to 0.14% for cement-lime mortar (Dubovoy 1990).
Appearance. Uniformity of color and shade of the mortar
jointsgreatly affects the overall appearance of a masonry
structure.Atmospheric conditions, admixtures, and initial rate of
absorption(suction) of the masonry units are some of the factors
affecting thecolor and shade of mortar joints. Others are
uniformity of proportionsof the mortar mix, water content, and time
of tooling the mortar joints.
Fig. 4. ASTM C 1072 bond wrench apparatus. (IMG13317)
* IRA is measured in g/min•30 in.2 (g/min•194 cm2)
Careful measurement of mortar materials andthorough mixing are
important to maintain uniformity from batch to batch and from dayto
day. Control of this uniformity becomesmore difficult with the
number of ingredientsto be combined at the mixer. Pigments, ifused,
will provide more uniform color if pre-mixed with a stock of cement
sufficient forthe needs of the whole project. In manyareas, colored
masonry cements are available;they provide better control over
color unifor-mity. Tooling of mortar joints at like degreesof
setting is important to ensure a uniformmortar shade in the
finished structure. If thejoint is tooled when the mortar is
relativelyhard, a darker shade results than if the jointsare tooled
when the mortar is relatively soft.Some masons consider mortar
joints ready fortooling after the mortar has stiffened but isstill
thumb-print hard, with the water sheengone. Tooling white cement
mortar withmetal tools may darken the joint. A glass orplastic
joint tool should be used.
Specifications and Selection of Types
Specifications. ASTM C 270, StandardSpecification for Mortar for
Unit Masonry,and CSA Standard A179, Mortar and Groutfor Unit
Masonry, are the main specificationdocuments in North America. ASTM
C 270 covers four types of mortars (Type M, S, N, or 0)while CSA
A179 defines two types of mortars**
(Type S and N). Current specifications formortars for
nonreinforced and reinforced unitmasonry are shown in Tables 1 and
2. Mortartypes are to be identified by either proportionor property
specifications, but not by both.An interplay of property and
proportion specifications is not intended or recognizedby the
The proportion specifications (Table 1) identi-fy mortar type
through various combinationsof portland or blended cement with
masonrycement, masonry cement singly, and combi-nations of portland
or blended cement andlime. The proportion specifications govern
when ASTM C 270 or CSA Standard A179 are referred to without noting
which specification—proportion or property—should be used.
Table 1. Proportion Specifications for Mortar
A. United States - ASTM C270
Parts by volume
Mortar Portland cement Masonry cement or Hydrated lime
Aggregatetype or blended cement mortar cement type or lime
M S N
1 -- -- 1 -- 41⁄2 to 6
M -- 1 -- -- -- 21⁄4 to 3
1 -- -- -- 1⁄4 213⁄16 to 33⁄4
1⁄2 -- -- 1 -- 33⁄8 to 41⁄2
S -- -- 1 -- -- 21⁄4 to 3
1 -- -- -- Over 1⁄4 to 1⁄2 *
-- -- -- 1 -- 21⁄4 to 3
N 1 -- -- -- Over 1⁄2 to 11⁄4 *
-- -- -- 1 -- 21⁄4 to 3
O 1 -- -- -- Over 11⁄4 to 21⁄2 *
B. Canada - CSA A179
Parts by volume
Mortar Portland cement Masonry cement or Hydrated lime
Aggregatetype or blended cement mortar cement type or lime
-- 1 -- -- 21⁄4 to 3
S 1⁄2 -- 1 -- 31⁄2 to 41⁄2
1 -- -- 1⁄2 31⁄2 to 41⁄2
-- -- 1 -- 21⁄4 to 3
N 1 -- -- 1 41⁄2 to 6
*The total aggregate shall be equal to not less than 21⁄4 and
not more than 3 times the sum of the volumes of the cement andlime
Notes: 1. Under both ASTM C270, Standard Specification for
Mortar for Unit Masonry, and CSA A179, Mortar and Grout forUnit
Masonry, aggregate is measured in a damp, loose condition and 1 ft3
of masonry sand by damp, loose volume is considered equal to 80 lb
of dry sand (in SI units 1 m3 of damp, loose sand is considered
equal to 1280 kg of dry sand).
2. Mortar should not contain more than one air-entraining
** Information on the traditional requirements for Type M, 0,
and K mortars and a descriptionof their uses is given in the
nonmandatory appendix A of CSA A179.
Mortar type classification under the property specifications
(Table 2)is dependent on the compressive strength of 2-in. (50-mm)
cubes,water retention, and air content, using standard laboratory
tests perASTM C 270 or CSA A179. These test requirements of the
propertyspecifications for laboratory mortar do not apply to
job-made mortar.Laboratory mortars are prepared with less water
than will be used onthe job. The standard consistency for
laboratory mortars is determinedusing a laboratory flow table (Fig.
5). In this test, a truncated cone ofmortar is subjected to
twenty-five 1⁄2-in. (12.7-mm) drops of a laboratoryflow table
plate. The diameter of the disturbed sample is comparedto the
original diameter of the conical sample. Allowable initial
flowranges from 105% to 115% for ASTM and 100% to 115% for CSA.This
consistency is not suitable for laying masonry units in the
field.Rather, it is intended to approximate the flow and properties
of fieldmixed mortar after it has been placed in contact with
absorptivemasonry units. Flow values of 130% to 150% are common for
theinitial consistency of mortar used in actual construction.
In the laboratory, the water retention limit is measured by a
flow-after-suction test, which simulates the action of absorptive
masonryunits on the plastic mortar. The test is described in C
1506, StandardTest Method for Water Retention of Hydraulic
Cement-Based Mortarsand Plasters and CSA A3004, Physical Test
Methods for CementitiousMaterials for Use in Concrete and Masonry
Cement. Upon performinga flow test before and after absorptive
suction on the mortar, theflow after suction must equal or exceed
75% or 70% of the originalflow for ASTM or CSA, respectively.
Once the proportions of cement, lime, and aggregate have
beenestablished in the laboratory for mortar meeting Table 2
propertyspecifications, the same proportions must be used in the
Mortar should be evaluated in the field according to ASTM C
780,Standard Test Method for Preconstruction and
ConstructionEvaluation of Mortars for Plain and Reinforced Unit
Masonry,or CSA A179, Mortar and Grout for Unit Masonry. The
provides test methods to ensure that the field mortar meets
therecipe that was selected from ASTM C270 or CSA A179
specifications.The test methods are equally effective whether
specifications werechosen based on proportions or properties (C 270
Table 1 or Table 2,respectively). Field quality control is based on
the mortar aggregateratio test and the mortar water content test.
The mortar aggregateratio test provides a means to identify,
measure, evaluate, and controldifferences which may be expected to
exist between laboratory andjobsite mortars. The water content test
provides information neededto calculate the mortar aggregate ratio.
Used together, they enableeffective quality control of field
mortars. Results are rapidly availableand allow for changes to
procedures to correct non-conforming mortars during the
When ASTM C 780 is to be used for quality control
testing,preconstruction testing using procedures described in the
standardmust be conducted to develop data that can serve as a
benchmarkfor evaluation of test results obtained during
construction (see PCA(1997) for further information on field
testing of masonry mortar).Unlike ASTM C 270, CSA A179 also has
compressive strengthrequirements (not shown in Table 2) for
job-prepared mortar proportioned according to property
ASTM C 780 provides guidance for compressive strength testing.
Itshould be recognized, however, that compressive strength
valuesdetermined on field mortars are generally lower than those
forlaboratory prepared mortars, and are not required or expected
tomeet the property specification requirements of Table 2.
Compressivestrengths of mortar cube specimens molded under field
test conditionsdo not represent the strength of the mortar in
place, nor are theyindicative of the compressive strength of the
masonry.* In addition, testresults are usually determined at 7 and
28 days, too late to enactconstruction procedures that might
correct the situation. For thesereasons, compressive strength
testing is not recommended for qualitycontrol in the field.
For the designer seeking data representative of the in-place
masonry,the most effective procedures are masonry assembly tests
such asASTM C 1314, the Standard Method for Constructing and
TestingMasonry Prisms Used to Determine Compliance with
SpecifiedCompressive Strength of Masonry. These assembly tests
indicate theinteraction between mortar and unit, quality of
workmanship, mortarconsistency, and numerous other characteristics
of the masonry.
The ratio of cementitious material to aggregate in the mixture
underthe property specifications may be less than under the
proportionspecifications. This is to encourage preconstruction
mortar testing;an economic reward is possible if less cement is
required for a mix tomeet the strength requirement of the property
specifications. In boththe property and proportion specifications,
the amount of water tobe used on the job is the maximum that will
produce a workable
Fig. 5. Flow test. (IMG14093)
* Mortar in the wall is much stronger than the tested strength
of the cube because the jointhas a smaller aspect ratio than the
cube and in-place mortar has a lower water-cementratio. Compressive
strength of masonry is a function of both the unit strength and
consistency during construction. This is unlike conventional
concretepractice where the water-cement ratio must be carefully
Selection. Once the design loads, type of structure, and
masonryunits have been determined, the mortar type can be selected.
No onemortar type will produce a mortar that rates the highest in
all desirableproperties. Adjustments in the mix to improve one
property often aremade at the expense of others. For this reason,
the properties ofeach mortar type should be evaluated, and the
mortar type chosenthat will best satisfy the end-use requirements.
See PCA (1998) foradditional guidance on selecting and specifying
The Masonry Standards Joint Committee documents—ACI
530/ASCE5/TMS 402, Building Code Requirements for Masonry
Structures(MSJC Code), and ACI 530. I/ASCE 6/TMS 602, Specification
forMasonry Structures (MSJC Specification)—have been adoptedby the
International Building Code and by the last published editions of
the BOCA National Building Code and the StandardBuilding Code. As a
result, many areas of the country now havesimilar requirements.
Specifiers should be familiar with both thedesign requirements of
the MSJC Code and the provisions of theMSJC Specification. The MSJC
Code makes several distinctions inthe structural characteristics of
masonry constructed using Type N mortar compared to that of masonry
constructed using Type S or Mmortar. In addition, for masonry
design that takes into consideration
the flexural tensile resistance of masonry, allowable flexural
tensilestresses are different for non-air-entrained portland
cement-lime ormortar cement mortars than for air-entrained portland
cement-lime ormasonry-cement mortars. The Uniform Building Code
(UBC) has similarprovisions, except that air-entrained portland
cement-lime mortarsare not specifically addressed. Mortar cement
mortars are used onan equivalent basis as cement-lime mortars. The
specifier should confirmthat mortar types and materials indicated
in project specificationsare consistent with structural design
requirements of the masonry.
In the United States, mortar is selected based on the
(desired)compressive strength of the masonry, type of masonry unit,
type andlocation of building segment, and conditions of the
loading, soil, andexposure. Table 3, adapted from ASTM C 270,
provides guidelines forselecting mortar for plain (nonreinforced)
masonry. For example, theguide recommends Type 0 mortar for
non-load-bearing walls, Type Nfor load-bearing walls and exterior
walls above grade, and Type S forexterior walls and masonry
applications at or below grade. Alternatemortar types are also
Special attention to mortar selection must be given when
severeexposure conditions, special masonry applications, or
reinforcedmasonry applications are considered. Type 0 mortar should
not beused in saturated freezing conditions. For severe frost
action or heavyloading, Type M mortar should be considered.
Table 2. Property Specifications for Laboratory-Prepared
A. United States
Minimum 28-day Maximum air content, %Mortar Mortar compressive
strength, Minimum water Masonry Mortar cement
specification type psi, (MPa) retention, % cement or
M 2500 (17.2) 75 18 12
ASTM C 270 S 1800 (12.4) 75 18 12
N 750 (5.2) 75 20 14
O 350 (2.4) 75 20 14
Minimum compressiveMortar Mortar strength, MPa Minimum water
specification type 7-day†† 28-day retention, %
CSA A179 S 7.5 12.5 70
N 3 5 70
* The total aggregate shall be equal to not less than 21⁄4 and
not more than 31⁄2 times the sum of the volumes of the cement and
** When structural reinforcement is incorporated in masonry
cement mortar, the maximum air content shall be 18%.
† When structural reinforcement is incorporated in mortar cement
or cement-lime mortar, the maximum air content shall be 12%.
†† If the mortar fails to meet the 7-day requirement but meets
the 28-day requirement, it shall be acceptable.
be used to improve freeze-thaw durability, although it may
reducebond and compressive strengths.
Mortar should also be compatible with the masonry unit. For
example,a masonry unit with a high rate of absorption is compatible
with amortar having a high water retentivity. Mortar strength
should neverbe greater than the masonry unit's strength. It is not
always necessaryto use Type M mortar for high-strength masonry,
because Type S canprovide comparable strength of masonry. Moreover,
Types S and Ngenerally have greater workability, water retention,
In Canada, Types S or N mortars are permitted for masonry
designedon the basis of engineering analysis and for masonry
designedaccording to empirical procedures. As previously noted,
Types M, 0,and K are not included in the body of the current
edition of CSA A179but are described in the nonmandatory Appendix A
of thatdocument. Types 0 and K are not allowed where the masonry is
tobe (1) directly in contact with soil, as in a foundation wall, or
(2)exposed to the weather on all sides, as in a parapet wall,
balustrade,chimney, or steps and landings. CSA (1997), CSA (1996),
and NRCC(1995) provide more information on mortar selection in
White and Colored Mortars
White and colored mortars can provide a color contrast or
harmonybetween masonry units and joints to create pleasing
architecturaleffects. White mortar is made with white masonry
cement, or withwhite portland cement and lime, and white sand. For
colored mortars,the use of white masonry cement or white portland
cement insteadof the normal gray cements not only produces cleaner,
brighter colors,but is essential for making pastel colors such as
buff, cream, ivory,pink, and rose.
Integrally colored mortar may be obtained through the use of
pigments,colored masonry cements, or colored sand. Brilliant or
intense colorsare generally not attainable in masonry mortars. The
color of themortar joints will depend not only on the pigment, but
also on thecementitious materials, aggregate, water-cement ratio,
Pigments must be thoroughly dispersed throughout the mix.
Todetermine if mixing is adequate, some of the mix is flattened
under atrowel. If streaks of color are present, additional mixing
is required.For best results, the pigment should be premixed with
the cement inlarge, controlled quantities. Alternately, colored
masonry cement isavailable in many areas in a range of stock
colors, and alleviates theneed for measuring and blending cements
with pigments on the job.Custom colors may be available from some
producers as well.
As a rule, pigments should be of mineral oxide compositionand
contain no dispersants that will slow or stop the portlandcement
hydration. Iron, manganese, chromium, and cobaltoxides have been
successfully used. Zinc and lead oxidesshould be avoided, because
they may react with the cement.Carbon black may be used as a
coloring agent to obtain darkgray or almost black mortar, but
lampblack should not beused. Carbon black should be limited to 1%
or 2% by weightof the cement for masonry cement or portland
cement-limemortars, respectively, since durability of this mortar
may belowered. In addition, the color of mortar using carbon
blackpigment rapidly fades with exposure to weathering.
Use only those pigments that have been found acceptable by
testing andexperience. The following is a guide to the selection of
Red, yellow, brown, black, or gray . . . . . . . . . . . . .Iron
Table 3. Guide for the Selection of Masonry Mortars (United
Mortar typeLocation Building segment Recommended Alternative
Exterior, above grade Load-bearing walls N S or M
Non-load-bearing walls O N or S
Parapet walls N S
Exterior, at or Foundation walls, S M or N†
below grade retaining walls, manholes,sewers, pavements,
Interior Load-bearing walls N S or M
Non-load-bearing partitions O N
*Adapted from ASTM C 270. This table does not provide for
specialized mortar uses, such as chimney, reinforced masonry, and
**Type 0 mortar is recommended for use where the masonry is
unlikely to be frozen when saturated or unlikely to be subjected to
high winds or other significant lateral loads. Type N or S mortar
should be used in other cases.
†Masonry exposed to weather in a nominally horizontal surface is
extremely vulnerable to weathering. Mortar for such masonry should
be selected with due caution.
Green . . . . . . . . . . . . . . . . . . . . . . . . . . . .
Blue . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
. . .Cobalt oxide
Only the minimum quantity of pigment that will produce the
desiredshade should be used. An excess of pigment, more than 10% of
theportland cement or 5% of the masonry cement by weight, may
bedetrimental to the strength and durability of the mortar. The
quantityof water used in mixing colored mortar should be accurately
controlled.The greater the water content, the lighter the color of
the mortar. Assuch, retempering or adding water to colored mortar
should be donecautiously. Mortar stiffness while tooling also has
an effect on color.
Variations in the color of materials are such as to make a
colorformula only approximate. Best results are obtained by
experiment.Test panels should be made with the same materials and
proportionsintended for use in the actual work and stored for about
5 daysunder conditions similar to those at the jobsite. Panels will
have adarker shade when wet than when dry.
Discoloration of colored mortar joints may be caused by
efflorescence,the formation of a white film on the surface. The
white deposits arecaused by soluble salts that have emerged from
below the surface,or by calcium hydroxide, which is liberated
during the setting of thecement, that subsequently combines with
atmospheric carbon dioxideto form carbonate compounds. Good
pigments do not effloresce orcontribute to efflorescence.
Efflorescence is more visible on a coloredsurface and may be
removed with water, stiff-bristle brush, a lightsandblasting, or
acid wash. See PCA (2002a) for more information.
Cementitious materials. Foremost among the factors that
contribute to good mortar is the quality of the mortar
ingredients.The following material specifications of ASTM or CSA
• Masonry cement—ASTM C 91 (Types M, S, or N); CSA A3002(Types S
• Mortar cement—ASTM C 1329 (Types M, S, or N); CSA A3002(MCN,
• Portland cement—ASTM C 150 (Types I, IA, II, IIA, III or
IIIA);CSA A3001 (Types GU, MS, HS, HE)
• Blended hydraulic cement—ASTM C 595 (Types IS, IS-A, IP,
IP-A,I(PM), or I(PM)-A)*
• Hydraulic cement—ASTM C 1157 (Types GU, MS, HS, HE)• Hydrated
lime for masonry purposes—ASTM C 207 (Types S,
SA, N, or NA)**
• Lime putty—ASTM C 1489Masonry sand. Since the quantity of sand
required to make 1 cu ft(0.0283 m3) of mortar may be as much as
0.99 cu ft (0.0280 m3), thesand has considerable influence on
mortar properties. Masonry sandfor mortar should comply with the
requirements of ASTM C 144,Standard Specification for Aggregate for
Masonry Mortar, for
* Slag cement Types S or SA can also be used but only according
to the property specifications.
** Types N and NA lime may be used only if tests or performance
records show that these limes are not detrimental to the soundness
Fig. 6. A colored mortar made with light red masonry cementpicks
up the earth tones of this brick, while a standard graymortar, also
made with masonry cement, complements the
concrete masonry units that it joins. (IMG14575)
construction within the United States and CSA A179 withinCanada.
These specifications include both natural and man-ufactured sands.
Sand should be clean, well graded, andmeet the gradation
requirements listed in Table 4.
Sands with less than 5% to 15% passing the Nos. 50(300 µm) and
100 (150 µm) sieves generally produce harsh or coarse mortars,
which possess poor workabilityand result in mortar joints with low
resistance to moisturepenetration. On the other hand, sands finer
than those permitted by the above specifications may yield mortars
withexcellent workability, but they may be weak and porous.
For mortar joints that are less than the conventional 3⁄8 in.(10
mm) thickness, 100% of the sand should pass the No.8 (2.36 mm)
sieve and 95% the No. 16 (1.18 mm) sieve.For joints thicker than
3⁄8 in. (10 mm), the mortar sandselected should have a fineness
modulus* approaching 2.5or a gradation within the limits of
concrete sands (fineaggregate) shown in ASTM C33, Standard
Specificationfor Concrete Aggregates, or CSA A23.1,
ConcreteMaterials and Methods of Concrete Construction.
All cementitious materials and aggregates should bestored in
such a manner as to prevent wetting, deterioration, or intru-sion
of foreign material. Brands of cementitious materials and thesource
of sand supply should remain the same throughout the entirejob.
Water. Water intended for use in mixing mortar should be clean
andfree of deleterious amounts of acids, alkalies, and organic
materials.Some potable waters contain appreciable amounts of
soluble saltssuch as sodium and potassium sulfate. These salts may
later contributeto efflorescence. Also, a water containing sugar
would retard the set.Thus, the water should be fit to drink, but
investigated if it containsalkalies, sulfates, or sugars.
Admixtures. Although water-reducers, accelerators, retarders,
andother admixtures are used in concrete construction, their use
inmasonry mortar may produce adverse effects on the normal
chemicalreaction between cement and water, especially during the
earlyperiods after mixing when water is needed for hydration of the
portlandcement. Hardened properties are also affected. ASTM C 270
indicatesthat admixtures should not be used in masonry mortar
unless specified.When they are specified and used, they should meet
the requirementsof ASTM C 1384, Standard Specification for
Admixtures for MasonryMortars. ASTM C 1384, which classifies
admixtures by their effect onperformance characteristics,
recognizes the following classifications:bond enhancers,
workability enhancers, set accelerators, set retarders,and water
Because there is no current standard test method for
determiningcorrosion potential of mortars toward embedded and
materials, a limit on chlorides is set. The MSJC Specification
limitsthe chloride content of admixtures to a maximum of 0.2%.
InCanada, CSA A179 does not permit the use of salts or chlorides
inany masonry containing connectors or reinforcement. ASTM C
1384establishes that the mortar admixture not add more than 65
ppm(0.0065%) water-soluble chloride or 90 ppm (0.0090%)
acid-solublechloride to the mortar’s overall chloride content.
Set-controlling admixtures have been reliably used to produce
extended lifemortar (see "Extended Life Mortar" section of this
publication). Regularretarders, as used in concrete, are
undesirable, because they reducestrength development and increase
the potential toward efflorescence.
Air-entrainment increases workability and freeze-thaw
durability.However, addition of an air-entraining admixture at the
mixer on ajobsite is not recommended, due to the sensitivity of the
admixtureand the likelihood of poor control in monitoring air
content.Materials with factory controlled amounts of air-entraining
agentsuch as masonry cement, mortar cement, air-entraining
portlandcement, or air-entraining lime, should be used if
air-entrainment isdesired. Also see "Cold-Weather Construction" and
"ModifiedMortars" sections of this publication.
Whenever admixtures are considered for use in masonry,
andexperience or performance records are not available, it is
recommendedthat the admixture be laboratory-tested in the
construction mortarsat the temperature extremes expected during
their use, and then jobsite-inspected to ensure their satisfactory
performance under theprevailing conditions.
Table 4. Aggregate Gradation for Masonry Mortar
Gradation specified, percent passing
Sieve size no. ASTM C144**
U.S. (Metric) Natural sand Manufactured sand
4 (4.75 mm) 100 100
8 (2.36 mm) 95 to 100 95 to 100
16 (1.18 mm) 10 to 100 70 to 100
30 (600 µm) 40 to 75 40 to 75
50 (300 µm) 10 to 35 20 to 40
100 (150 µm) 2 to 15 10 to 25
200 (75 µm) 0 to 5 0 to 10
** Additional requirements: Not more than 50% shall be retained
between any two sievesizes, nor more than 25% between No. 50 and
No. 100 (300 µm and 150 µm) sieve, sizes.Where an aggregate fails
to meet the gradation limit specified, it may be used if themasonry
mortar will comply with the property specification of ASTM C 270
* Fineness modulus equals the sum of the cumulative percentages
retained on the standardsieves, divided by 100. The higher the
fineness modulus, the coarser the sand.
Measuring Mortar Materials
Measurement of masonry mortar ingredients should be completed in
amanner that will ensure the uniformity of mix proportions, yields,
work-ability, and mortar color from batch to batch. Aggregate
proportions aregenerally expressed in terms of loose volume, but
experience has shownthat the amount of sand can vary due to
Fig. 7 shows how loose sand with varying amounts of
surfacemoisture occupies different volumes. Fig. 8 has the same
data inanother form for fine sand and shows the density of the
sand.While dry sand or saturated sand typically has a unit weight
of over 100 lb/ft3 (1600 kg/m3), damp loose sand generally
containsapproximately 80 lb/ft3 (1280 kg/m3) of dry sand plus the
weight ofthe water. ASTM C 270 and CSA A179 procedures for
proportioningmortar ingredients are based on the premise that sand
will be usedin a damp and loose condition at the construction site.
Thus, to conform with specification requirements and to assure
consistentvolume batching, sand stock should be maintained in a
damp, loosecondition. The sand pile at the construction site should
be coveredto reduce evaporation and provide protection from rain or
Ordinary sands will absorb water amounting approximately to
0.4%to 2.3% of the weight of the sand. In the field, damp sands
usuallyhave 4% to 8% moisture, so most of the water is on the
surface ofthe sand.
Mortar ingredients other than sand are often sold in bags
labeledonly by weight. Since mortar is proportioned by volume, it
is necessaryto know the following data:
Unit weight, lb/ft3 (kg/m3)
Portland cement 94 (1500)
Masonry cement* 70 to 90 (1120 to 1440)
Hydrated lime (dry) 40 (640)
Lime putty (wet density) 80 to 90 (1280 to 1440)
*See printed net weight on bag.
Sand is commonly added to the mortar mixer using a
shovel.However, some positive control should be established to
assure thatthe proper volume of sand is used. That can be
accomplished byperiodically checking the required shovel count with
a box of knownvolume, using that measuring box to add the sand to
the mixer, orusing calibrated buckets to measure sand added to the
mixer. (Acubic foot box is a common and practical size.) When a
measuringbox is used, a hinged attachment to the mortar mixer can
be constructedto facilitate one-man operation. When buckets are
used, they shouldbe calibrated to determine actual volume capacity.
For example: if itis determined that buckets being used for
proportioning have avolume capacity of exactly five gallons, then,
since 1 cu ft is equal to7.48 gal, 3 cu ft of sand is 22.44 gal or
41⁄2 five-gallon buckets ofsand. To obtain a mortar having a 3 to 1
volume proportion of sand
to cementitious materials, 41⁄2 buckets of sand would be added
to themixer for each bag of masonry cement or cubic foot of cement
pluslime used in the mortar batch.
00 5 10 15 20
Percent of moisture added by weightto dry, rodded sand
Most probable moisturecontent of sand at site
Masonry sandF/M – 2.30
Most probable moisturecontent of sand at site
0 5 10 15 20
Percent of moisture added by weightto dry, loose sand
Fig. 7. Volume of loose, damp sand.
Fig. 8. Weight of loose, damp sand.
To obtain good workability and other desirable properties of
plasticmasonry mortar, the ingredients must be thoroughly
Mixing by machine. With the possible exception of very
smalljobs, mortar should be machine-mixed. A typical mortar mixer
(Fig. 9)has a capacity of 4 cu ft to 7 cu ft (0.1 m3 to 0.2 m3).
Conventionalmortar mixers are of rotating-spiral or paddle-blade
design with tiltingdrum. After all batched materials are together,
they should be mixedfrom 3 to 5 minutes. A shorter mixing time may
result in non-uniformity, poor workability, low water retention,
and less-than-optimumair content. Longer mixing times may adversely
affect the air contents of mortars containing air-entraining
cements, particularlyduring cool or cold weather. Longer mixing
times may also reducethe strength of the mortar.
Batching procedures will vary with individual preferences.
Experience has shown that good results can be obtained when about
three-fourthsof the required water, one-half of the sand, and all
the cementitiousmaterials are briefly mixed together. The balance
of the sand is thencharged and the remaining water added. The
amount of water addedshould be the maximum that is consistent with
Mixing is carried out most effectively when the mixer is charged
toits design capacity. Overloading can impair mixing efficiency
andmortar uniformity. The mixer drum should be completely
emptybefore charging the next batch.
Mixing by hand. When hand-mixing of mortar becomes necessary,as
on small jobs, all the dry materials should be mixed together
byhoe, working first from one end of a mortar box (or
wheelbarrow)and then from the other. Next, two-thirds to
three-fourths of therequired water is mixed in with the hoe and the
mixing continued asabove until the batch is uniformly wet.
Additional water is carefullymixed in until the desired workability
is attained. The batch shouldbe allowed to stand for approximately
5 minutes and then thoroughlyremixed with the hoe.
Retempering. Fresh mortar should be prepared at the rate used,so
that its workability remains fairly consistent throughout the
day.Mortar that sits unused for long periods of time tends to dry
out andstiffen. Loss of water by absorption and evaporation on a
dry day canbe reduced by wetting the mortarboard and covering the
mortar inthe mortar box, wheelbarrow, or tub.
If necessary to restore workability, mortar may be retempered
byadding water; thorough remixing is then necessary. Although
smalladditions of water may slightly reduce the compressive
strength ofthe mortar, the result is acceptable. Masonry built
using plastic mortarhas a better bond strength than masonry built
using dry, stiff mortar.
Mortar that has stiffened because of hydration should be
discarded.Since it is difficult to determine by sight or feel
whether mortar stiffeningis due to evaporation or hydration, the
most practical method ofdetermining the suitability of mortar is on
the basis of time elapsedafter mixing. Mortar should be used within
21⁄2 hours after mixing.
Retemper colored mortar cautiously to avoid color changes.
Watercontent and stiffness of mortar during tooling can also affect
The key to successful construction of masonry in any weather—hot
or cold—lies in advanced planning and careful
preparation.All-weather construction involves some change in
procedures andadditional equipment and supplies. Both hot and cold
weather significantly influence the entire masonry construction
industry. Hot-weather problems often have been encountered but not
recognized,resulting in some sacrifice of quality or increase in
construction costs.On the other hand, greater extension of the
construction season intothe winter months in recent years has
resulted in better utilization ofmanpower and encouraged innovative
Fig. 9. For best results, the mortar should be mixedwith a power
Fig. 10. To restore workability, mortar may be
Hot-weather construction. Hot weather poses some specialproblems
for masonry construction. These arise, in general, from
highertemperatures of materials and equipment and more rapid
evaporationof the water required for cement hydration. Other
factors contributingto the problems include wind velocity, relative
humidity, and sunshine.
As the temperature of mortar increases, there are several
accompanyingchanges in its physical properties:
• Workability is lessened; or, for a given workability, more
• A given amount of air-entraining agent yields less entrained
• Initial set and final set occur earlier, and evaporation rates
• Depending on the surface characteristics, temperature,
andmoisture content of the masonry units, their absorption
ofmoisture from the mortar may be faster.
The MSJC Specification defines hot weather construction as
occurring when ambient temperature exceeds 100°F or 90°F with a
wind velocity greater than 8 mph (38°C or 32°C at 13 km/h in CSA
A371). Under such conditions masonry units are to be set withinone
minute of spreading mortar and open mortar beds are to be limitedto
no more than 4 ft (1.2 m). Additional measures such as
storingmasonry materials and equipment in cool shaded areas,
constructingwind breaks, cooling mixing water, and controlling
evaporation ratesby covering or fogging masonry may be helpful.
High absorption claymasonry units should be wetted before use to
reduce initial rates ofabsorption. Concrete masonry units should
not be wetted before use.
Cold-weather construction. Ideal temperature for the placement
and curing of masonry mortar is in the range of 70°F ±10°F (21.1°C
± 5.5°C). In cold weather, defined as 40°F (4.4°C)and below, mortar
materials need to be heated; otherwise, the mortaris likely to
exhibit slower setting times and lower early strengths.
Water acts as a lubricant in the plastic mortar and is required
forhydration of the portland cement contained in the mortar.
Whilemortar stiffens as water is absorbed by units and evaporates,
thehardening of mortar is a result of the reaction between the
portlandcement and water. This reaction rate is temperature
dependent andis slowed or stopped when the cement paste temperature
is below40°F (4.4°C). When masonry construction is carried on
during periodsof cold weather, proper facilities should be
available for preparingthe mortar and protecting the fresh masonry
work during the criticalearly curing stages, when the free water
content of mortar is high(above 6%), to avoid disruptive expansion
in the mortar due tofreezing. Sufficient heat must be provided to
ensure hydration of thecement. After combining all ingredients,
mortar temperature isrequired to be within the range of 40°F to
120°F (United States), or20°C to 50°C (Canada). Mortar temperatures
in excess of 120°F(50°C) may cause excessively fast hardening, with
resultant loss ofcompressive and bond strength. Table 5 shows
requirements atvarious cold-weather temperatures for heating of
Figs. 11a, b. Warm sand and a continuous supply of hot watermay
be needed when cold weather arrives. Sand can be heatedover fire in
a pipe (above) and water can be heated in metaldrums (below).
Table 5a. Cold Weather Construction Requirements for Work in
Progress (United States)*
Temperature (ambient) Cold weather procedures
Above 40°F (4.4°C) No special requirements.
Below 40°F (4.4°C) Do not lay glass unit masonry.
32°F to 40°F Heat sand or mixing water to produce mortar
temperature between 40°F and 120°F (4.4°C and 48.9°C) (0 to 4.4°C)
at the time of mixing.
Heat materials for grout only if they are below 32°F (0°C).
25°F to 32°F Heat sand or mixing water to produce mortar
temperature between 40°F and 120°F (4.4°C and 48.9°C) (-3.9°C to
0°C) at the time of mixing. Keep mortar above freezing until used
Heat materials to produce grout temperature between 70°F and
120°F (21.1°C and 48.9°C) at the time of mixing. Keep grout
temperature above 70°F (21.1°C) at the time of placement.
20°F to 25°F In addition to requirements for 25°F to 32°F
(-3.9°C to 0°C), heat masonry surfaces under construction (-6.7°C
to -3.9°C) to 40°F (4.4°C) and use wind breaks or enclosures when
the wind velocity exceeds 15 mph (24 km/h).
Heat masonry to a minimum of 40°F (4.4°C) prior to grouting.
20°F (-6.7°C) In addition to all of the above requirements,
provide an enclosure and auxiliary heat to keep airand below
temperature above 32°F (0°C) within the enclosure.
*Adapted from recommendations of the International Masonry
Industry All-Weather Council and requirements of Masonry Standards
Joint Committee (MSJC) Specification for MasonryStructures (ACI
530.1-02/ASCE 6-02/TMS 602-02).
Table 5b. Protection Requirements for Newly Completed Masonry
Temperature Cold weather procedures(minimum for grouted;mean
daily for ungrouted)
Above 40°F (4.4°C) No special requirements.
25°F to 40°F Cover newly constructed masonry with a
weather-resistive membrane for 24 hours(-3.9°C to 4.4°C) after
20°F to 25°F Cover newly constructed masonry with
weather-resistive insulating blankets (or equal protection)(-6.7°C
to -3.9°C) for 24 hours after being completed.
Extend the time period to 48 hours for grouted masonry, unless
the only cement used in the grout is Type III portland cement.
20°F (-6.7°C) Keep newly constructed masonry above 32°F (0°C)
for at least 24 hours after being completed.and below Use heated
enclosures, electric heating blankets, infrared lamps, or other
Extend the time period to 48 hours for grouted masonry, unless
the only cement used in the grout is Type III portland cement.
*Adapted from recommendations of the International Masonry
Industry All-Weather Council and requirements of Masonry Standards
Joint Committee (MSJC) Specification for MasonryStructures (ACI
530.1-02/ASCE 6-02/TMS 602-02).
protection of construction. Table 6 shows the same information
formasonry in Canada.
The use of Type Ill portland cement or non-chloride based
acceleratorsmay be helpful to increase rates of early-age strength
developmentof masonry mortar. Accelerators normally used include
soluble carbonates, silicates and fluosilicates, aluminous cements,
calciumaluminate, and some organic compounds such as
triethanolamine.Calcium chloride, a common accelerator for use in
concrete, can haveadverse side effects such as corrosion of
embedded metal. Therefore,the MSJC Specification prohibits its use
as an admixture for mortar.
Admixtures are not effective in lowering the freezing point of
mortarsto any appreciable degree. The quantity of such materials
would beso large that mortar strength and other desirable
properties wouldbe seriously impaired. Therefore the use of
accelerators does noteliminate the need to observe recommended cold
weather practicesor the need to protect newly constructed masonry
Table 6a. Cold Weather Construction Requirements for Work in
Air temperature Cold weather procedures
0°C to 4°C Heat sand or mixing water to a minimum of 20°C and a
maximum of 70°C.
-4°C to 0°C Heat sand or mixing water to a minimum of 20°C and a
maximum of 70°C.
-7°C to -4°C Heat sand or mixing water to a minimum of 20°C and
a maximum of 70°C. Provide heat on both sides of walls under
construction. Use windbreaks when wind exceeds 25 km/h.
-7°C and below Heat sand or mixing water to a minimum of 20°C
and a maximum of 70°C. Provide enclosures and supplementary heat to
maintain air temperature about 0°C. The temperature of the unit
when laid should not be less than 7°C.
Note: Grout should be placed at a minimum temperature of 20°C
and a maximum temperature of 50°C, then maintained about 0°C for 24
hours following placement of the grout.
*Source: Canadian Standards Association (CSA 1994).
Table 6b. Protection Requirements for Newly Completed Masonry
Mean dailyair temperature Cold weather procedures
0°C to 4°C Protect masonry from rain of snow for 24 hours.
-4°C to 0°C Completely cover masonry for 24 hours.
-7°C to -4°C Completely cover masonry for 24 hours with
-7°C and below Maintain masonry above 0°C for 24 hours by
enclosure and supplementary heat.
Note: The amount of insulation required to properly cure masonry
in cold weather shall be determined on the basis of the expected
air temperature and wind velocity (wind-chill factor)and the size
and shape of the structure.
*Source: Canadian Standards Association (CSA 1994).
Fig. 12. Enclosure and heating of a work area protects
materials,workers, and installed masonry from severe weather.
Special Mortar Production Techniques
Packaged Dry Mortar Materials. Packaged, combined, drymortar
ingredients have been available since 1936. The bag of drymortar
contains cementitious materials and dry sand accuratelyproportioned
and blended at a manufacturing plant. Only water andmixing are
required at the project. The mortar is available in Types M,S, and
N. Packaged dry mortar is very useful on small jobs, such
asprojects needing 1 cu ft to 5 cu ft (0.03 m3 to 0.14 m3) of
mortar, orjobs with limited space to store mortar ingredients. This
mortarshould meet the requirements of ASTM C 387, Specification
forPackaged, Dry, Combined Materials for Mortar and Concrete.ASTM C
387 contains property specifications similar to those in Table
Dry-batching. In dry-batching, the cementitious materials
anddried sand are accurately weighed and blended at a central
plantbefore delivery to the site in a sealed truck, where the
mixture isconveyed into a sealed, weathertight hopper. When the
masoncontractor is ready for mortar, he has only to add the water
and mix.In a variation of this basic concept, the premixed dry
may be delivered to the jobsite in bulk-pack bags. The process
ofdry-batching mortar ingredients alleviates the need to adjust the
mixfor moisture content of the sand and ensures consistent portions
ofsand and cementitious materials.
Silo-Mixed Mortar. Silo mixers consist of a screw (auger)
mixerthat is fed dry mortar ingredients for a silo. Single bin
silos usepreblended mortar ingredients, whereas multi-compartment
siloshouse mortar ingredients separately. For example, two
compartmentsilos have one compartment for sand and one compartment
The silo is filled with mortar ingredients at a central plant,
deliveredto the jobsite by truck, and erected. Mortar ingredients
are accuratelyweighed and preblended as needed at the plant to meet
the specificproject requirements. On site, the unit needs only to
be connected toa pressurized water source and electricity. Mixing
at the project iscontrolled by a computer, so the contractor merely
presses a buttonwhen mortar is needed. The mortar is usually
deposited into aportable tub or wheelbarrow for distribution at the
As with the dry-batching techniques mentioned previously, silo
mixedmortars provide accurate batching of mortar materials, reduce
jobsitewaste, and require very little jobsite space.
Fig. 13. The storage bin/batcher at this central plant stores
individual mortar ingredients (masonry cement, portland cement,
lime, and sand) in separate compartments. The computer
controlledplant batches the dry ingredients by weight and dry
them prior to discharge into the silos. (IMG14081)
Fig. 14. When connected to electricity and water at the
jobsite,the silo mixer is ready to produce mortar as needed.
Extended Life Mortar. Extended life mortar, also known
asready-mixed mortar, is batched at a central location, usually a
readymixed concrete or mortar batch plant, mixed in the plant, and
deliveredto the jobsite in trowel-ready condition. Extended life
mortar is madewith essentially the same ingredients as conventional
mortar, exceptthat the mortar contains a special retarding,
set-controlling admixturethat keeps the mortar plastic and workable
for a period of more than2-1⁄2 hours, usually 24 to 36 hours.
Conventional mortar ingredients(cement, lime, and sand) in
conventional proportions are combinedwith a retarding,
set-controlling admixture and enough water to provide the desired
field consistency. The ingredients are mixed at acentral location,
using either stationary mixers or truck mixers. Animportant
advantage of extended life mortar is that the ingredients
are accurately measured by mass (weight) or by metering
devices,thereby producing more uniform mixes closely meeting design
speci-fications. The volumetric methods used for conventionally
preparedfield mortar can be less accurate.
The design of extended life mortar is usually based on a
performancespecification and, therefore, proper preliminary
laboratory testing isrequired to determine ingredient proportions.
Once proportions areestablished, they should not be changed
throughout the job exceptfor admixture adjustments required to
compensate for temperaturechanges to maintain a consistent setting
period or board life.
Extended life mortar should meet the requirements of ASTM C
1142,Specification for Extended Life Mortar for Unit Masonry.
Themortar types are designated as Type RM, RS, RN, and RO. Table
7lists the property specifications for these mortars.
Trowel-ready mortar is delivered to the jobsite in ready mix
trucks,mortar transports, mortar containers, or hoppers (see Fig.
15).The mortar is stored in a protected metal or plastic
(1⁄4 to 1⁄3 cubic yard or cubic meter) to minimize evaporation
and avoidtemp-erature extremes. The retarding, set-controlling
admixturedelays the initial hydration of the cement, causing the
mortar toremain plastic and workable for 24 to 36 hours.
Extended life mortar is used the same way as conventional mortar
inreinforced and nonreinforced masonry. If the mortar stiffens due
toevaporation or absorption of water, the mortar can be
retemperedwith additional water to restore workability. However,
the mortarshould not be used beyond its predetermined life
When the mortar is placed between masonry units, the units
absorbwater from the mortar, thereby removing the set-controlling
from solution, at which time the extended life mortarproceeds to
set like normal mortar. Therefore,masonry walls can be constructed
at the samerate as walls with normal mortar. Like normalmortar,
sufficient water should be present in themortar to develop proper
strength gain; however,special precautions should be taken to
reduceevaporation on hot and windy days.
Extended life mortar should be used with cautionwith
nonabsorbent units such as glazed unitsand glass block. Extended
life mortar should beretarded for no more than 10 hours for
The cautions and concerns of using conventionalmortar are also
applicable to extended life mortar.Special information about the
use of extended lifemortar, including jobsite storage
requirements,useful life, and allowable extent of
retempering,should be provided by the producer.
Specific controls and procedures must be carefully followed in
orderto obtain a successful mortar mix with an extended plastic
life.Among these are careful mix design and careful batching
Table 7. Property Specifications for Extended Life Mortar*
Mortar Average Minimum water Maximum airtype compressive
retention, % content, %†
strength at 28 days,minimum psi (MPa)**
RM 2500 (17.2) 75 18
RS 1800 (12.4) 75 18
RN 750 (5.2) 75 18
RO 350 (2.4) 75 18
*Adapted from ASTM C 1142.
**The strength values are standard 2-in. (50-mm) cube strength
values. Intermediate values may be specified in accordance with
project requirements. Cylindrical specimens (2x4 in. or 3x6 in.,
[50x100mm or 75x150mm])can also be used as long as their strength
relationship to cube strength is documented by the producer with
testdata. The 28-day time period starts when the specimens are
cast, not when the mortar is initially mixed.
†When structural reinforcement is incorporated in mortar, the
maximum air content shall be 12% or bond strength test shall be
provided to justify higher air content.
Fig. 15. Extended life, or ready-mixed, mortar is often
deliveredin mortar containers (tubs) or a flatbed truck. The
containers are unloaded and left at the jobsite. (IMG14082)
To maintain quality and consistent behavior of the mortar,
sources ofsupply for the original mix ingredients should not
deviate. Bond andcompressive strength, water permeance, and other
properties ofextended life mortar are generally equivalent to the
properties ofconventional mortar. The applicable laboratory, batch
plant, and fieldquality assurance tests in ASTM C 1142 and C 780 or
CSA A179should be used and a qualified inspector should be present
to perform the tests. Specimens for comp-ressive strength tests
shouldbe moved from the field to the laboratory after the mortar
hasundergone final set and the specimens are four or more days
Masonry walls built with extended life mortar can be loaded
atabout the same time as walls built with normal mortar, except
whenused with low absorptive units or wet units. If the loading
period isof concern, ASTM C 1314 prism tests can be performed to
determineproper loading time.
Modified Mortars. Occasions arise when modified masonry
mortarmay be considered beneficial. Modified mortars are
conventionalmasonry mortars altered by either the addition of an
admixture at themixing location or the replacement of one of the
basic mortar ingre-dients. Benefits are appraised from laboratory
testing of comparativemortars and testing of walls containing
ASTM C 270 recognizes admixtures when specified, but the
presentspecification does not provide guidance toward accept/reject
criteria.Some of the concerns with respect to the indiscriminate
use ofadmixtures are discussed in the appendix to ASTM C 270.
Modifiers considered for use in the masonry industry are
essentiallysimilar to those used in the concrete industry. Concrete
technology,however, must be tempered for masonry industry
applications andassessment of benefits. Modifiers having varying
degrees of acceptancein the masonry industry are classified in
Selection and use of a mortar modifier should be based on field
performance and laboratory testing. Manufacturers of mortar
modifiersshould be asked to provide data supporting their claims as
to theperformance of their products under the anticipated climatic
conditionsthat will prevail during use. Modifiers, be they
admixtures orreplacements, must not be used indiscriminately.
Table 8. Modifiers–Benefits and Concerns
Modifier Primary benefits Possible Concerns
Air-entraining Freeze-thaw durability, Effect on compressive and
Bonding Wall tensile (and flexural) Reduced workability,bond
strength bond strength regression upon wetting,
Plasticizer Workability, economy Effect on hardened physical
propertiesunder field conditions
Set accelerator Early strength Effectiveness at cold
temperatures,development corrosive properties, effect on
potential of masonry
Set retarder Workability retention Effect on strength
development, effect on efflorescence potential of masonry
Water reducer Strength, workability Effect on strength
development under field conditions with absorptive units
Water repellent Weather resistance Effectiveness over time
Pozzolanic Increased density Effect on plastic and hardenedand
strength physical properties under field conditions,
Color Aesthetic versatility Effect on physical properties,color
stability over time
CSA, Masonry Design and Construction for Buildings, CSA
StandardS304-1977, Canadian Standards Association, Rexdale,
CSA, Masonry Construction for Buildings, CSA Standard
A371,Canadian Standards Association, Rexdale, Ontario, 1994.
CSA, Masonry Design for Buildings (Limit States Design),CSA
Standard S304.1-94, Canadian Standards Association,Rexdale,
CSA, Mortar and Grout for Unit Masonry, CSA Standard
A179,Canadian Standards Association, Rexdale, Ontario, 1999.
Dubovoy, Val S., Evaluation of Selected Properties of
MasonryMortars—Special Testing Program, Portland CementAssociation,
Dubovoy, V. S., and Ribar, J. W., Masonry Cement
Mortars-ALaboratory Investigation, Research and Development
BulletinRD0095, PCA, Skokie, IL, 1990.
Fishburn, C. C., "Effect of Mortar Properties on Strength
ofMasonry," National Bureau of Standards Monograph 36,National
Bureau of Standards, Washington, 1961.
Isberner 1974a, Isberner, Albert W., Properties of Masonry
CementMortars, Research and Development Bulletin RD019,
PortlandCement Association, 1974.
Isberner 1974b, Isberner, Albert W., Specifications and
Selection ofMaterials for Masonry Mortars and Grouts, Research
andDevelopment Bulletin RD024, Portland Cement Association,
Melander, J. M., and Conway, J. T., "Compressive and Bond
Strengthsof Portland Cement – Lime Mortars," Masonry: Design
andConstruction, Problems and Repairs - STP1180, ASTM,
WestConshohocken, Pennsylvania, 1993, pages 105-120.
Melander, J. M., and Ghosh, S. K., "Development of
Specifications forMortar Cement," Masonry: Esthetics, Engineering,
andEconomy, ASTM STP 1246, D. H. Taubert and J. T. Conway,
Eds.,ASTM, West Conshohocken, PA, 1996, pages 88-99.
MIC, Hot and Cold Weather Masonry Construction, MasonryIndustry
Council, Lombard, Illinois, 1999. (Available from PCA as
MSJC Code, Building Code Requirements for Masonry Structures(ACI
530-02/ASCE 5-02/TMS 402-02), Specifications forMasonry Structures
(ACI 530.1 -02/ASCE 6-02/TMS 602-02),Commentary on Building Code
Requirements for MasonryStructures (ACI 530-02/ASCE5-02/TMS 402-02)
andCommentary on Specifications for Masonry
Structures(AC1530.1-02/ASCE 6-02/TMS 602-02), American
ConcreteInstitute, Farmington Hills, Michigan, American Society of
CivilEngineers, New York, and The Masonry Society, Boulder,
NBS, American Standard Building Code Requirements forMasonry
(A41.1), National Bureau of Standards, MiscellaneousPublication
211, American National Standards Institute,New York, 1954.
NCMA, Extended Life Mortars, National Concrete
MasonryAssociation , NCMA TEK 9-2A, National Concrete
MasonryAssociation, Herndon, Virginia, 1997.
BIA, "Ready-Mix Mortars," Engineering and Research Digest,Brick
Industry Association, Reston, Virginia, 1983.
NRCC, "Plain and Reinforced Masonry," Supplement No. 4 to
theNational Building Code of Canada, National Research Councilof
Canada, Ottawa, Ont., 1975.
NRCC, National Building Code of Canada 1995, National
ResearchCouncil of Canada, Ottawa, Ont., 1995.
Panarese, Kosmatka, and Randall 1991, Panarese, W. C.,
Kosmatka,S. H., and Randall, F. A,, Jr., Concrete Masonry Handbook
forArchitects, Engineers, Builders, EB008, Portland
PCA 1986a, "Tuckpointing," Concrete Technology Today, Vol. 7,No.
3, PL863, Portland Cement Association, 1986.
PCA 1986b, "Ready Mixed Mortar Update", Concrete
TechnologyToday, Vol. 7, No. 4, PL864, Portland Cement Association,
PCA 1992a, Recommended Practices for Laying Concrete
Block,PA043, Portland Cement Association, 1992.
PCA 1992b, Trowel Tips: Tuckpointing, IS240, Portland
PCA, Masonry Cement Mortars, IS181, Portland CementAssociation,
PCA, Trowel Tips: Field Testing Masonry Mortar, IS242,
PortlandCement Association, 1997.
PCA, Selecting and Specifying Mortar and Grout for UnitMasonry,
lS275, Portland Cement Association, 1998.
PCA 2002a, Efflorescence, IS239, Portland Cement Association,
PCA 2002b, Masonry Cement; Product Data Sheet, IS282,Portland
Cement Association, 2002.
PCA 2002c, Mortar Cement: Product Data Sheet, IS281,
PortlandCement Association, 2002.
Ritchie, T., and Davison, J. I., "Factors Affecting Bond
Strength andResistance to Moisture Penetration of Brick
Masonry,"Symposium on Masonry Testing - STP320, ASTM ,
WestConshohocken, Pennsylvania, 1963.
PCA R&D Serial No. 2226
Portland Cement Association ("PCA") is a not-for-profit
organization and provides this publi-cation solely for the
continuing education of qualified professionals. THIS
PUBLICATIONSHOULD ONLY BE USED BY QUALIFIED PROFESSIONALS who
possess all required license(s),who are competent to evaluate the
significance and limitations of the information providedherein, and
who accept total responsibility for the application of this
information. OTHERREADERS SHOULD OBTAIN ASSISTANCE FROM A QUALIFIED
PROFESSIONAL BEFORE PRO-CEEDING.
PCA AND ITS MEMBERS MAKE NO EXPRESS OR IMPLIED WARRANTY WITH
RESPECT TO THISPUBLICATION OR ANY INFORMATION CONTAINED HEREIN. IN
PARTICULAR, NO WARRANTYIS MADE OF MERCHANTABILITY OR FITNESS FOR A
PARTICULAR PURPOSE. PCA AND ITSMEMBERS DISCLAIM ANY PRODUCT
LIABILITY (INCLUDING WITHOUT LIMITATION ANYSTRICT LIABILITY IN
TORT) IN CONNECTION WITH THIS PUBLICATION OR ANY
This publication is intended SOLELY for use by PROFESSIONAL
PERSONNEL who are compe-tent to evaluate the significance and
limitations of the information provided herein, and whowill accept
total responsibility for the application of this information. The
Portland CementAssociation DISCLAIMS any and all RESPONSIBILITY and
LIABILITY for the accuracy of and theapplication of the information
contained in this publication to the full extent permitted by
An organization of cement companies toimprove and extend the
uses of portlandcement and concrete through market development,
engineering, research,education, and public affairs work.
© 2004 Portland Cement Association.All rights reserved.
American Society for Testing and Materials
C 5-03 Standard Specification for Quicklime for Structural
C 91-03a Standard Specification for Masonry Cement
C 144-03 Standard Specification for Aggregate for Masonry
C 150-02a Standard Specification for Portland Cement
C 151-00 Standard Test Method for Autoclave Expansion of
C 207-91(1997) Standard Specification for Hydrated Lime
C 270-03 Standard Specification for Mortar for Unit Masonry
C 387-00e1 Standard Specification for Packaged, Dry,
CombinedMaterials for Mortar and Concrete
C 595-03 Standard Specification for Blended Hydraulic
C 780-02 Standard Test Method for Preconstruction and
ConstructionEvaluation of Mortars for Plain and Reinforced Unit
C 952-02 Standard Test Method for Bond Strength of Mortar
C 1012-02 Standard Test Method for Length Change of
Hydraulic-Cement Mortars Exposed to a Sulfate Solution
C 1072-00a Standard Test Method for Measurement of
MasonryFlexural Bond Strength
C 1142-95(2001) Standard Specification for Extended Life Mortar
C 1148-92a(2002) Standard Test Method for Measuring the
DryingShrinkage of Masonry Mortar
C 1157-02 Standard Performance Specification for Hydraulic
C 1314-02a Standard Test Method for Compressive Strength
C 1329-03a Standard Specification for Mortar Cement
C 1384-02a Standard Specification for Admixtures for
C 1489-01 Standard Specification for Lime Putty for
C 1506-03 Standard Test Method for Water Retention of
HydraulicCement-Based Mortars and Plasters
E 72-02 Standard Test Methods of Conducting Strength Tests
ofPanels for Building Construction
E 518-02 Standard Test Methods for Flexural Bond Strength
Canadian Standards Association
A179-94 (R1999) Mortar and Grout for Unit Masonry (1999)
A371-94 (R1999) Masonry Construction for Buildings (1999)
A3001-03 Cementitious Materials for Use in Concrete (2003)
A3002-03 Masonry Cement (2003)
A3003-03 Chemical Test Methods for Cementitious Materials for
Usein Concrete and Masonry Cement (2003)
A3004-03 Physical Test Methods for Cementitious Materials for
Usein Concrete and Masonry Cement (2003)
A3005-03 Test Equipment and Materials for Cementitious
Materialsfor Use in Concrete and Masonry Cement (2003)
S304 Masonry Design and Construction for Buildings (1997)
S304.1 Masonry Design for Buildings (Limit States Design)